Dear Label_Name,

Greetings! I hope you are well.

I am writing on behalf of an international publishing house, Science and Education Publishing, USA (http://www.sciepub.com).

Science and Education Publishing (SciEP) is a multidisciplinary open access publisher of Journals covering the fields of Science, Technology and Medicine. All SciEP publications are subject to high-quality peer review, editorial and production processes and are freely available online.

Welcome to the April, 2013 edition of SciEP newsletter, providing monthly summaries of articles on science & education related topics of interest to scientist and professionals. The mission of our journals is to provide an open access forum for publishing new findings on issues pertinent to scientific and academic field. We also invite you to submit original research papers, review articles, short reports, or case studies are considered for publication in our Multidisciplinary Journals.

American Journal of Public Health Research
DOI: 10.12691/ajphr-1-1-3

The Implementation of a Tele-Homecare System with Service Oriented Architecture and HL7 Message Transmission Standard
Ching-Sung Wang

American Journal of Medical and Biological Research
DOI: 10.12691/ajmbr-1-1-2

The Influence of Ethanol on Pyruvate Kinases Activity in Vivo, in Vitro, in Silico
Lelevich Sergey Vladimirovich, Khrustalev Vladislav Victorovich, Barkovsky Eugene Victorovich, Shedogubova Tatyana Aleksandrovna

American Journal of Medical Sciences and Medicine
DOI: 10.12691/ajmsm-1-1-1

Clinical and Histological Features in Wegener Granulomatosis
Li Cavoli Gioacchino, Passantino Rita, Bono Luisa, Tortorici Calogera, Ferrantelli Angelo, Giammarresi Carlo, Rotolo Ugo

American Journal of Infectious Diseases and Microbiology
DOI: 10.12691/ajidm-1-1-2

The Curse of Lymphatic Filariasis: Would the Continual Use of Diethylcarbamazine Eliminate this Scourge in Papua New Guinea?
Anne Lanham, Lillian Mwanri

We have released issues of some journals on February 2013.
American Journal of Public Health Research
American Journal of Medical Sciences and Medicine
American Journal of Medical and Biological Research
American Journal of Pharmacological Sciences
American Journal of Clinical Medicine Research
American Journal of Nursing Research
American Journal of Cancer Prevention
American Journal of Medicine Studies
American Journal of Infectious Diseases and Microbiology
American Journal of Cardiovascular Disease Research
American Journal of Biomedical Research
American Journal of Mechanical Engineering
American Journal of Microbiological Research
Journal of Preventive Medicine
American Journal of Food and Nutrition
American Journal of Hypertension Research
American Journal of Sports Science and Medicine
Journal of Cancer Research and Treatment
American Journal of Zoological Research
Journal of Biomedical Engineering and Technology
American Journal of Microbiological Research
Biomedical Science and Engineering

We are pleased to announce that submissions are now being accepted for peer review for all the journals across all our subject areas in SciEP.

Please submit your manuscript via our online submission system:
http://www.sciepub.com/author/signin

To unsubscribe from our mailing list, please click on the following link: unsubscribe

I am looking forward to hearing from you.

Kind regards,

David Rain
Email:join@sciepub.com
Science and Education Publishing (http://www.sciepub.com)

Effect of Hydrophilic Amide Monomers on Dentin Bonding Strength

Mustafa Duzyol*, Sevim Atilan Yavuz, Zeyneb Merve Ozdemir, Esra Duzyol

Department of Restorative Dentistry, Faculty of Dentistry, Istanbul Medeniyet University, Istanbul, Turkey

Abstract: Objective: The aim of this study was to compare the shear bond strength (SBS) to dentin of one-step bonding agent containing hydrophilic amide monomers (HMA) and 10-Methacryloyloxydecyl dihydrogen phosphate (MDP) with one-step bonding agent containing only MDP. Materials and Methods: 20 human third molar teeth randomly were divided into two groups. Teeth was abraded with a SiC disc (Carbimet, Bisco Inc., Schaumburg, USA) to be under 1 mm of enamel-dentin junction. The dentin surface of each teeth were etched with %37 phosphoric acid for 15 s and then rinsed with water spray for 10 s and after that air dried. Cylinders of composite (Clearfil Majesty Posterior, Kuraray Noritake Inc, Okuyama, Japan) were bonded using 2 dental bonding agents. Group A used bonding agent containing HMA+MDP (Clearfil Universal Quick bond, Kuraray America, Inc. New York/NY, USA) and Group B used bonding agent containing only MDP (Clearfil S3 Bond plus, Kuraray America, Inc. New York/NY, USA) applied in accordance with the manufacturer's instructions. The speciemens were stored for 24 h in 37°C water and thermocycled between 5 and 55 C water with a 20 s dwell time for 5000 cycles. They were then submitted to a shear bond test with a universal testing machine (AGS-X, Shimadzu, Kyoto, Japan) with a 100 N load cell at 1 mm/min. The values of SBS were analyzed with ANOVA/Tukey’s test. Results: Group A was 35,96±5,47 MPa and B was 24,25±7,5 MPa There was a statistical difference between the two bonding agents (p<0.05). Group A was significantly higher than Group B. Conclusions: According to this study, bonding agents containing which type of monomers may be one of the important factors influencing dentin bond strength. When bonding agents with hydrophilic amide monomers are used, it has showed higher shear bond strength.

Keywords: hydrophilic amide monomers, dentin bonding, shear bonding strength, polymerization time

Received March 01, 2020; Revised April 05, 2020; Accepted April 16, 2020

Citation: Mustafa Duzyol, Sevim Atilan Yavuz, Zeyneb Merve Ozdemir, Esra Duzyol, Effect of Hydrophilic Amide Monomers on Dentin Bonding Strength. International Journal of Dental Sciences and Research, 8 (3). 72-74. January 2020. doi:10.12691/ijdsr-8-3-3

1. Introduction

For dental tissue bonding, dentin bonding systems consist primarily of synthetic resin monomers that can partially leak into the demineralized dental structure. These systems include hydrophilic and/or hydrophobic monomers, photo-initiators, stabilizers, solvents and inorganic fillers [1]. Depending on the mode of operation, the current adhesives can be used according to two major adhesion strategies. These are: "etch & rinse" (ER) in which phosphoric acid is to be etching; and "self-etching" (SE) where no etching is needed [2]. Selective etching is an adhesion strategy that combines ER and SE with acid application only to enamel and applies multi-mode or universal adhesive to both enamel and dentine [3,4].

Self-adhesives are commonly used due to their user-friendly, simple application. [5] Today, the use of aggressive self-adhesives is gradually decreasing due to its comparatively weak dentin bond strength [6]. Less aggressive self-etching adhesives have eventually become the major goods. [5] However, these adhesives cannot completely dissolve the dentin smear layer. They will provide hybridization with dentin smear layer to form a 'resin-smear layer complex' [7]. Therefore, the weakest connection exists at the resin-dentin interface when using these adhesives. [8].

Universal adhesives are the latest generation dentin bonding system. [9] Universal adhesives are designed to bond to dental structures by both chemical and micromechanical mechanisms due to the existence of certain functional monomers, such as 10-methacryloyloxydecyl dihydrogen phosphate (MDP). [10,11,12] These added monomers, on the one side, form a chemical bond with calcium in hydroxyapatite crystals, while at the same time forming a hybrid layer polymerized on the other ends. [13]

The purpose of this study is to compare the bonding strength of dentin bonding systems containing hydrophilic amide monomers and containing 10-Methacryloiloxidesyl dihydrogen phosphate (MDP) to dentin tissue in an attempt to shed light on their clinical use.

2. Material and Methods

In this study, 20 non-carious third molar teeth were used. To create a smooth occlusal dentin surface, the occlusal enamel was removed with a SiC disc (Carbimet, Bisco Inc., USA), below the 1 mm enamel-dentin boundary. Teeth were embedded in cylindrical acryl blocks with exposed dentin surfaces exposed. Dentin surfaces were abraded with 600 gr sandpaper and a standard smear layer was created. The samples were randomly divided into 2 groups (n = 10).

Universal adhesive systems were applied to the dentin surfaces prepared according to the manufacturer's instructions (Table 1). It was polymerized with a powerful LED light source (ValoLed, Ultradent Products Inc, Utah, USA) in the required time. All groups were restored with 4 x 4 mm sized nanohybrid composite discs (Clearfil Majesty Posterior, Kuraray, Japan).

Samples were kept in 37 °C water for 24 hours and a thermal cycle of 5 to 55 °C was performed for 5000 cycles with a 20 second standby time. They were subjected to shear bond strength testing with a universal tester (AGS-X, Shimadzu, Japan). The breaker tip was positioned on the composite parallel to the bonding surface. The composites were broken by applying shear force at a speed of 0.5 mm / min. Maximum strength values were determined and the results were calculated in MPa. The statistical analysis of the obtained data was done with One Way Variance Analysis and Tukey HSD.

Table 1. The materials and forms of application

Table 2. The mean of shear bond strength (MPa)

Figure 1. Fracture patterns

3. Results

Shear bond strength is shown in Table 2.

The mean shear bond strength of Clearfil Universal Bond Rapid was measured at 35.96 ± 5.47 MPa and the mean shear bond strength of Clearfil S3 Bond was measured at 24.25 ± 7.5 MPa. As a consequence of the statistical assessment, the discrepancy was important when comparing the bond strength between groups (p<0.05). The forms of refraction were calculated by a light microscope. (Figure 1).

4. Discussion

In this study, when the shear bond strength of the universal adhesive systems was compared, it was seen that the materials had different results despite having a similar application procedure.

Universal systems are one-step self-etch systems. Self-etch primers also produce an acidic monomer that dissolves the coating layer and also demineralizes the dentin. The variations in bond strength between bonding structures can be due to various acidic monomers in the substance of the products. [14] Therefore, in our study, bonding systems with the same acidic monomers were used.

Poggio et al. [5] stated that the pH value of universal bonding systems does not substantially influence the shear bond strength of the enamel and dentin surfaces. It may be attributed to the significant effect of the pH concentration and the formation of the 10-methacryloloyloxidesyl dihydrogen phosphate (MDP) universal bonding systems. [16]. At the other hand, Nishiyama et al. [17] quantitatively investigated the effects of MDP at universal bonding systems without MDP-based2-hydroxyethyl methacrylate (HEMA). These study showed that HEMA, a hydrophilic monomer, increases the bond strength with MDP. [17]

HEMA is a monomer seen in a variety of fields today, including contact lenses. It is also used as a monomer with high water absorption in universal bonding agents. Although this feature facilitates the attachment to dentin, it also causes the appearance of a "water-tree" which reduces the binding strength in the long term. [18] The amide monomers in Clearfil Universal Bond Quick have quick penetration of the dentin surface while reducing the harmful effects of HEMA. That is why Clearfil Universal Bond Quick offers greater shear bond power in our research.

Universal bonding systems are preferred in clinical applications due to their additional applications and reduced time loss. Clearfil Universal Bond Quick fulfills one of the preferred reasons for universal bonding systems, as it does not require waiting time after application and polymerizes with 1500 mW / cm2 in 5 seconds. [19]

5. Conclusion

According to this study, the content of hydrophilic monomers is an important factor in the bond strength of dentin bonding systems. Dentin bonding system containing hydrophilic amide monomers showed shorter working time and higher shear bond strength.

References

[1]   | Van Landuyt KL, Snauwaert J, De Munck et al. Systematic review of the chemical composition of contemporary dental adhesives. Biomaterials 2007; 28: 3757-85.
[2]   | Sezinando A. Looking for the ideal adhesive-a review, Revista Portuguesa de Estomatologia. Med Dentária e Cir Maxilofac 2014; 55: 194-206.
[3]   | Frankenberger R, Lohbauer U, Roggendorf MJet al.. Selective enamel etching reconsidered: better than etch-and-rinse and self-etch. J Adhes Dent 2008; 10: 339-44.
[4]   | Feltrin Antoniazzi B, Ferreira Nicoloso G, Larissa Lenzi T et al.. Selective acid etching improves the bond strength of universal adhesive to sound and demineralized enamel of primary teeth. J Adhes Dent 2016; 18.
[5]   | Samimi, P., Ghodrati, M., Shirban, F et al. Comparison of the dentin bond strength of two self-etch adhesives after prolonged air-drying and additional light-curing. J. Dent. 2017; 14, 292-298.
[6]   | Shirai, K., De Munck, J., Yoshida, Y. et al. Effect of cavity configuration and aging on the bonding effectiveness of six adhesives to dentin. Dent. Mater. 2015; 21, 110-124.
[7]   | Mine, A., De Munck, J., Cardoso, M.V et al. Dentin- smear remains at self-etch adhesive interface. Dent. Mater. 2014;30, 1147-1153.
[8]   | Alshaikh, K.H., Hamama, H.H.H., Mahmoud, S.H. Effect of smear layer deproteinization on bonding of self-etch adhesives to dentin: a systematic review and meta-analysis. Restor. Dent. Endod. 2018; 43, e14.
[9]   | de Goes MF, Shinohara MS, Freitas MS. Performance of a new one-step multi-mode adhesive on etched vs non-etched enamel on bond strength and interfacial mor- phology. J Adhes Dent 2014; 16: 243-50.
[10]   | Hanabusa M, Mine A, Kuboki T, Momoi Yet al. Bonding effectiveness of a new ‘multi-mode’adhesive to enamel and dentine. J Dent 2012; 40: 475-84.
[11]   | Munoz MA, Sezinando A, Luque-Martinez Iet al. Influence of a hydrophobic resin coating on the bonding efficacy of three universal adhesives. J Dent 2014; 42: 595-602.
[12]   | Wagner A, Wendler M, Petschelt A et al.. Bonding performance of universal adhesives in different etching modes. J Dent 2014; 42: 800-7.
[13]   | Van Landuyt KL, De Munck J, Snauwaert J et al. Monomer-solvent phase separation in one-step self-etch adhesives. J Dent Res. 2005; 84(2): 183-188.
[14]   | Van Meerbeek B, De Munck J, Yoshida Y et al. Buonocore memorial lecture. Adhesion to enamel and dentin: current status and future challenges. Oper Dent. 2003; 28(3): 215-235.
[15]   | Poggio C., Beltrami R., Scribante A. et al. Chiesa, Shear bond strength of one-step self-etch adhesives: pH influence, Dent. Res. J. 2015; 209-214.
[16]   | Lührs A.K., Guhr S., Schilke R., et al. Shear bond strength of self-etch adhesives to enamel with additional phosphoric acid etching, Oper. Dent. 2008; 155-162.
[17]   | Iwai H, Nishiyama N, Effect of calcium salt of functional monomer on bonding performance, J. Dent. Res. 2012; 1043-1048.
[18]   | Yokota Y., Nishiyama N., Determination of molecular species of calcium salt of MDP produced through decalcification of enamel and dentin by MDP-based one-step adhesive, Dent. Mater. J. 2015; 270-279.
[19]   | Schouten, P. Super stick, super quick!. Brit. Dent. J, 2017, 223.8: 614.